Intrinsic defect energies of lithium hydride and lithium
Ravindra Pandeyt and A M Stoneham
Theoretical Physics Division, AERE Harwell, Oxon OX11 O R A , UK
Received 4 March 1985
Abstract. A theoretical study has been made of the defect structure of lithium hydride and lithium deuteride. A potential model is obtained describing the statics and dynamics of these crystals. Intrinsic defect energies are calculated using the Harwell HADES program which is based on a generalised Mott-Littleton method. The results are in good agreement with the experimental data, and suggest that the vacancy and interstitial migration mechanisms of
anions and cations are all comparable in their contribution to ionic conduction.
The hydride and deuteride of lithium represent two of the simplest ionic crystals and, apart from their intrinsic scientific interest, are also representatives of the hydrides that may have important technological applications such as in fuel hydrogen storage. These crystals possess the rocksalt structure, with only four electrons in the primitive unit cell.
In the ideal fully ionic state, both the cation and anion have the closed-shell configuration of the helium atom. In addition, these crystals exhibit alarge isotope effect in both cation (6Li and 'Li) and anion (lH, 2H, 3H) sublattices.
In a series of studies, Pretzel and his co-workers described the preparation and properties of lithium hydride (LiH) and lithium deuteride (LiD) single crystals (Pretzel et a1 (1962) and the earlier papers from the same group cited in this reference). They proposed models for some of the irradiation-induced point defects analogous to those in the alkali halide family using the optical absorption and electron paramagnetic resonance techniques. Anderson and Luty (1983) reported the luminescence emission produced by unspecified defects in these crystals, whereas Miki and Ikeya (1982) explained the results of a thermoluminescence study of irradiated crystals by proposing the formation of Frenkel pairs and the mobility of hydrogen interstitials at extremely low temperatures. From ionic conductivity curves, the Schottky pair formation energy and cation migration energy have been deduced (Ikeya 1977, Varotsos and Mourikis 1974). However, the Frenkel pair formation energies and anion migration energy are still unknown. Theor- etical studies, on the other hand, have been limited to lattice dynamics calculations (Dyck and Jex 1981, Verble et a1 1968). Thus, the results obtained from experimental and theoretical studies represent a far from satisfactory knowledge of the intrinsic defect structure of these crystals.
t Physics Department, University of Manitoba. Winnipeg (Manitoba), Canada R3T 2N2.
5290 R Pandey and A M Stoneham
In an attempt to expand our physical understanding of the defect properties of these crystals, we have made a theoretic study which is based on lattice simulation techniques that have proved reliable for ionic and semi-ionic crystals. Our analysis intentionally concentrates on the parallel with alkali halides. Clearly, other classes of defect are possible, e.g. ones based on molecular ions such as Li: and H:
,or centres based on atomic species Ho or Lio; Ho, in particular, is known as a substitutional and interstitial defect in alkali halides. We find, nevertheless, that the bulk of the existing experimental data can be understood quantitatively within the framework of Schottky and Frenkel disorder.
2. Theoretical methods
In the present study, the intrinsic defect structure of the lattice has been simulated using the HADES code (Lidiard and Norgett 1972, Norgett 1974) which divides the lattice into two regions: an inner region I immediately surrounding the defect, where the lattice configuration is evaluated explicitly using painvise potentials which represent the ionic interactions, and an outer region
I1which can be treated by the Mott-Littleton approxi- mation using information on macroscopic response functions, namely the elastic and dielectric constants of the lattice. This code has been successfully applied to a wide variety of defect calculations in alkali and alkaline-earth halides, alkali, alkaline-earth, transition-metal and actinide oxides (Mackrodt (1982) and references therein), zinc selenide (Harding and Stoneham 1982) and calcium sulphide (Pandey and Harding 1984).
We take a fully ionic model based on Li+ and H-/D- ions. Such a model is supported by the Hartree-Fock calculations by Dovesi et a1 (1984) and it is also consistent with much work on hydrogen defect centres in alkali halides (see, e.g., Stoneham (1975), ch 20). The value we use, Z = 1, within a shell model contrasts with the value Z = 0.875 used by Wilson and Johnson (1970), who combined a rigid-ion model with non-radial forces. The fits to perfect-crystal data are comparable in success; however, the use of 2 = 1 is more transparent physically and avoids many problems associated with the definition of the energies of charged defects.
The ionic interactions can be represented as the sum of long-range Coulomb inter- actions and short-range non-coulombic interactions caused by the overlap of the electron clouds of the two ions. We use a pair potential description of the short-range potential which is a simple analytical expression of the Born-Mayer form:
V , ( x > = A , exP(-x/P,). (1)
This may be supplemented by short-range attractive terms, that is, terms in x - 6 and x - ~ , often (but without good reason) attributed to ‘dispersion forces’; we shall include only thex? part. We use the shell model, originally proposed by Dick and Overhauser (1958) to simulate the ionic polarisation. In this model, the ionic polarisation is described by the displacement of a massless charged shell from a massive charged core, the two being connected by a harmonic spring. This allows dielectric properties of the crystal to be simulated accurately. The inter-ionic potential energy may therefore be expressed as a sum of painvise terms of the form
q J r , W , ,
+Y , Y , e 2 / / r
-r,) is the position of ion core j relative to ion core z,
W ,and W, the shell- core displacements, Y , and Y, the shell charges, K , and K, the spring constants, Z , and Z, the core charges of ions i and j , e the electronic charge, U the volume and VI, the short-
range part, assumed to act between the shells only.
The lattice potential energy contains the parameters that are to be determined. There are three short-range parts of the potential, VHH, VLILl and VLIH for LiH crystal and VDD, VLIL, and VrlD for LiD crystal. These potentials have been obtained as described below.
(i) V,, and VDD (the anion-anion short-range interactions) are obtained by using the theoretical models developed by Wedepohl (1967) and Gordon and Kim (1972). These models are based on the density functional treatment of the uniform electron gas. Here, the electronic structure of the H- ion in the Madelung potential field is calculated to obtain the ionic wavefunctions. Then this is pairwise superimposed, leading to inter- ionic pair interaction on the basis of the assumption that the charge densities of two isolated ions are unchanged when they are brought together, the resultant charge density being a simple superposition of the two. The computer program for this procedure is given by Harding and Harker (1982).
(ii) VLILl (the cation-cation short-range interaction) is taken to be independent of the crystal environment. Since this interaction is small at Li-Li separation, this assumption should not cause significant error. We have taken VLILl from the shell model of lithium fluoride (Catlow et a1 1977) which has nearly the same lattice spacing as that of both LiH and LiD
(iii) We use an empirical method to obtain VLIH and VLID (the cation-anion short- range interactions). In this method, short-range parameters are determined in such a way that the model potential reproduces the observed macroscopic crystal data, namely the cohesive energy, lattice spacing, elastic constants and dielectric constants. This method has been successfully applied for a wide range of halides, oxides and sulphides. Note here that the short-range potential includes a part due to the difference between D and H zero-point motion. This dynamical component can, we find, be chosen to represent well the perfect-crystal properties of both LiH and LiD. We are, however, making the assumption that the same dynamical potential is transferable, i.e. it will
Table 1. Parameters of the short-range potential V,, = A , exp(-r/p,) - C,,r-', together with values for the shell charge and spring constant,
A , Potential (eV)
VH,/VDD 6611.11 0.1315 0.98
VI.,,, 1153.80 0.1364 0.0
VL,H 188.57 0.3215 0.0
VL,, 18.46 0.3197 0.0
Spring constant Shell charge, e (eV
LiH Li- 0.998 40.08
H - - 1.005 4.24
LID Li' 0.998 40.99
RPandey and A M Stoneham
describe short-range interactions near defects as well as in the perfect solid. R Ball, J H
Harding and A M Stoneham (unpublished work) are developing a self-consistent phonons code to verify assumptions like this.
The resulting potentials are given in table 1. The values of A and p for Li-Li and Li- H(D) are similar to those of Wilson and Johnson (1970; in this comparison we consider their spherically averaged potentials). Our H-H (D-D) potential is repulsive, however, whereas theirs is attractive with shorter range.
It is interesting that the values of p for the LiH and LiD interactions are both about
A,i.e. in line with values for many ionic crystals. This is also consistent with values for other hydride-metal short-range interactions deduced from local mode frequencies of defects (by E Wade and A M Stoneham in unpublished work performed in 1979) and from the combination of hydride phonon data and local mode frequencies (Browne 1982).
3. Results and discussion
3.1. The perfect crystal
The calculated and the observed properties of LiH and LiD are listed in tables 2 and 3 respectively. It can be seen that they are reproduced quite well for all but Ci2, which by virtue of the pairwise interaction of the ions is inevitably overestimated. The Cauchy violation is, in fact especially large in LiH and LiD and can only be partly accounted for even by long-range three-centre potentials (Wendel and Zeyher 1980) although the Dyck and Jex (1981) deformation dipole model is able to give a good fit with 13 adjustable parameters. Likewise, the Jaswal andDilly (1977) 9-parameter fit gave reasonable lattice dynamics. However, these workers discuss only harmonic properties and do not provide a potential suitable for defect modelling. The Wilson and Johnson (1970) potential gives somewhat better values for Cl2 than ours, although only at the expense of less good values of the lattice parameter (their Model I) or cohesive energy (their Model 11).
We have tested the reliability of our potential model by calculating the phonon dispersion curves in the principal symmetry directions using the lattice dynamics package
Table 2. Properties of lithium hydride.
Calculated Observed (i) Lattice constant
(A)2.0417 2.0417a (ii) Cohesive energy (eV) -10.36 -9.44a (iii) Elastic constants
(10l2 dyn cm-2)
Cl1 7.98 7.41 2 0.2b
C!2 4.59 1.42 5 0.03
C44 4.57 4.84 ? 0.18
EO 13.92 12.9 t 0.5'
E, 3.32 3.61 t 0.5
(iv) Dielectric constants
(vi) Melting point (K) - 961'
a Pretzel eta1 (1962).
Table 3. Properties of lithium deuteride.
Calculated Observed (i) Lattice constant
(ii) Cohesive energy (eV) -10.43 (iii) Elastic constants
(10l2 dyn cm-2)
(iv) Dielectric constants
(v) Melting point (K)
7.68 t 0.2b 1.51
*0.03 4.94 2 0.18 14.0 2 0.5'
3.63 2 0.5 951' a Pretzel et a1 (1962).
James and Kheyrandish (1982) Brodsky and Burstein (1967).
developed by Sangster and Rowel1 (in 1983 (unpublished)) from the Harwell PHONONS program. The calculated dispersion curves are shown in figure 1 along with the observed spectra from an inelastic neutron scattering experiment for LiD crystal (experimental data are available for LiD only). We also have compared the frequency ratio o(LiH)/ w(LiD) with those from the lattice dynamics calculations of Verble er a1 (1968), based on a seven-parameter shell model fitted to neutron data on LiD in table
4.The overall agreement seems surprisingly good, keeping in mind the simplicity of our model. We may therefore conclude that our potentials, although simplified, provide a good approximate description of the harmonic statics and dynamics of LiH and LiD crystals.
0.8 0.6 0.4 0.2 0.1 0.2 0.3 0.4 1
R e d u c e d w a v e - v e c t o r , g
5294 R Pandey and A M Stoneham
Table 4. Calculated frequency ratios o(LiH)/w(LiD) for
r-,X- and L-point phonons of LiH and LiD
Calculated frequency ratios
Present study Verble et a1 (1968)
LO 1.35 1.38 1.43 1.33 1.39 1.40
TO 1.36 1.42 1.44 1.33 1.39 1.40
-1.04 0.99 - 0.99 0.97
3.2. Defect energies
In table 5 we present our calculated defect formation energies in these crystals. The energies appear to be in good agreement with the experimental values. We define the formation energy of avacancy as that required to remove a lattice ion to infinity, allowing the remaining lattice to relax to equilibrium. Likewise, the interstitial formation energy is that involved in bringing an ion from infinity to an interstitial site with corresponding relaxation of the surrounding lattice. The Schottky pair formation energy (E,) is then the sum of the energies of formation of isolated cation and anion vacancies, reduced by the energy of the removed ions placed at the surface, which is given in terms of the cohesive energy. The Frenkel pair energy
(EF)is the energy of formation of an isolated vacancy and an isolated interstitial. The antisite defect is either a Li+ ion at an H- site or a D- ion at a Li' site. Table 5 also contains the energies for the antisite defect pair, predicting that such defects are unlikely to be observed in these crystals in the form
+Li+H). However, we have not looked at possibilities like
H i ior ( H l ) L i , nor at
molecular species like HY in cation-anion divacancies (note that HLi reacting with a host
H- ion produces
H iin a divacancy).
The Schottky pair formation energy of LiH is greater than that of LiD which is in line with the usual rule that the formation energy increases with the increase in crystal melting point. Our calculation clearly shows the isotope effect in these crystals, subject
to our earlier remarks about transferability of potentials. The calculated formation energy of a Schottky pair is somewhat less than that of either Frenkel pair, thereby
Table 5. Intrinsic defect energies (eV)
Calculated Observed Calculated Observed Schottky pair 2.42 2.30 2 0.3a 2.29 2.40 iz O . O l b
*O . O l b
anion 2.70 - 2.61 -
cation 2.72 - 2.65 -
Antisite pair 7.81
a Ikeya (1977).
suggesting that vacancies, rather than interstitials, will be the most common defect species in both the crystals. However, interstitial defects prove to have a lower motion energy, and several mechanisms may contribute to ionic conduction.
We have calculated the activation energies for the migration of both anions and cations by vacancy and interstitial mechanisms. The activation energy is the energy of the saddle-point configuration relative to the isolated vacancy or interstitial. The saddle- point configuration consists of either a face-centred interstitial ion and two adjacent vacancies in the (110) direction for the vacancy mechanism, or a single face-centred ion for the interstitial mechanism. Note that these are classical (saddle-point) configurations rather than those for the small-polaron model used for H in metals (Flynn and Stoneham 1970). A corresponding calculation with the small-polaron model is possible, and is planned for later work; it will certainly be necessary if we are to interpret data on muon spin rotation. The calculated classical results are given in table 6 with the appropriate experimental results, and predict nearly the same activation energies for migration for both of the ions in these crystals.
Table 6 . Activation energies for migration ( e v ) .
Vacancy mechanism Interstitial mechanism Calculated Observed Calculated Observed LiH
Li' 0.42 0.54 2 0.02" 0.17
H- 0.40 - 0.19
Li' 0.33 0.52 t O.Olb 0.18 -
a Ikeya (1977).
Varotsos and Mourikis (1974).
The experimental value of about 0.5 eV has been reported for the migration of a cation vacancy. Our calculated energies are lower than this value in both the crystals. However, the analysis of the conductivity curves has been made by assuming that the mobile species are cation vacancies which occur as extrinsic defects due to the presence of divalent cations in the lattice (Ikeya 1977, Varotsos and Mourikis 1974). The exper- imental value is therefore the activation energy in the presence of associated impurities in the lattice, whereas the calculated energy is for free cation-vacancy migration. Thus, a lower calculated activation energy would be expected (see, e.g., Mackrodt 1982) as obtained in the present case.
5296 R Pandey and A M Stoneham
Table 7. The Arrhenius energy of migration ( e v ) . (The Arrhenius energy is the slope of the ionic conductivity curve and, in an intrinsic region of a crystal, is half of the Schottky pair formation energy plus the vacancy migration energy for a vacancy mode of migration (Case I) or half of the Frenkel pair formation energy plus the interstitial migration energy for an interstitial mode of migration (Case 11)).
Case I (vacancy) Case I1 (interstitial) LiH 1.70 2 0 . l a Li- 1.63 1.53
1.720 2 0.005b H- 1.61 1.54 LiD 1.695 ?0.005b Li' 1.47 1.51
D- 1.46 1.47
a Ikeya (1977).
Varotsos and Mourikis (1974).
a nearly linear conductivity curve which could scarcely be resolved in the analysis of conductivity curves.
In summary, we have obtained an apparently reliable potential model for LiH and LiD crystals and have predicted that both the interstitial and vacancy modes of migration are important for ionic conduction in these crystals. The relative contributions from both anions and cations to the conductivity in the intrinsic region is found here to be almost independent of the temperature.
The authors are grateful to Dr J H Harding and Professor J Vail for useful discussions. One of us (RP) acknowledges financial support from A E R E Harwell and NSERC Canada.
Anderson A and Luty F 1983 Phys. R e v . B 28 3415
Brodsky M H and Burstein E 1967 J . Phys. Chem. Soli& 28 1655 Browne A M 1982 P h D Thesis University of Oxford
Catlow C R A , Diller K M and Norgett M J 1977 J . Phys. C: Solid Stare Phys. 10 1395 Dick B G and Overhauser A W 1958 Phys. R e v . 112 90
Dovesi R , Ermondi C , Ferrero E, Pissani C and Roetti C 1984 Phys. R e v . B 29 3591 Duck W and Jex H 1981 J . Phys. C: Solid State Phys. 14 4193
Flynn C P and Stoneham A M 1970 Phys. R e v . B 13966 Gordon R G and Kim Y S 1972 J . Chem. Phys. 56 3122 Harding J H and Harker A H 1982 AERE Report R10425
Ikeya M 1977 J . Phys. Soc. Japan 42 168
James B Wand Kheyrandish H 1982 J . Phys. C: Solid State Phys. 15 6321 Jaswal S S and Dilly V D 1977 Phys. Reu. B 15 2366
Lidiard A B and Norgett M J 1972 Computarional Solid Stare Physics ed. F Herman, N W Dalton and R G Mackrodt W C 1982 Computer Simulation of Solids ed. C R A Catlow and W C Mackrodt (New York: iMiki T and Ikeya M 1982 J . Phys. Soc. Japan 51 2862
Norgett M J 1974 A E R E Report R7650
Pandey R and Harding J H 1984 Phil. Mag. B 49 135
Pretzel F E , Gritton G V, Rushing C C, Friauf R .I, Lewis W B and Waldstein P 1962J. Phys. Chem. Solids Stoneham A M 1975 Theory of Defects in Solids (Oxford: OUP)
Varotsos P A and Mourikis S 1974 Phys. Rev. B 10 5220 Verble J L, Warren J L and Yarnell J L 1968 Phys. Reu. 168 980 Wedepohl P T 1967 Proc. Phys. Soc. 92 79
Wendel H and Zeyher R 1980 Phys. Reu. B 21 5544 Wilson W D and Johnson R A 1970 Phys. Reu. B 13510
Kochler (New York: Plenum) p 385 Springer) p 175